Output from "TOTOPOL", (version 1.92, 17 Jul 2017, Mike Treacy).

Report for the framework in file "public/tmp/tmp_194_6_103630358_fvAKY2.cif"

There are 144 T-atoms per unit cell
There are 288 O-atoms per unit cell

Framework density = 19.73 T-atoms per nm^3
Material density = 1.969 grams per cm^3 (excluding extra-framework material)
-------------------------------------------------------------------
-------------------------- T-O Analysis ---------------------------
-------------------------------------------------------------------
[Si] Ideal SiO distance = 1.610 Angstrom
T1  -- O1  = 1.5829 Angstrom
T1  -- O2  = 1.6218 Angstrom
T1  -- O3  = 1.6558 Angstrom
T1  -- O4  = 1.6612 Angstrom
      mean = 1.6304 Angstrom
        t1 = 0.049836  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.059712  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T2  -- O3  = 1.6127 Angstrom
T2  -- O5  = 1.5654 Angstrom
T2  -- O6  = 1.6836 Angstrom
T2  -- O7  = 1.5753 Angstrom
      mean = 1.6092 Angstrom
        t1 = 0.060609  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.082811  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T3  -- O4  = 1.6543 Angstrom
T3  -- O8  = 1.6536 Angstrom
T3  -- O9  = 1.6279 Angstrom
T3  -- O10 = 1.7434 Angstrom
      mean = 1.6698 Angstrom
        t1 = 0.049750  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.029341  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T4  -- O6  = 1.5629 Angstrom
T4  -- O7  = 1.5651 Angstrom
T4  -- O11 = 1.6840 Angstrom
T4  -- O12 = 1.7199 Angstrom
      mean = 1.6330 Angstrom
        t1 = 0.078329  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.059273  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T5  -- O10 = 1.6662 Angstrom
T5  -- O12 = 1.5542 Angstrom
T5  -- O13 = 1.6691 Angstrom
T5  -- O14 = 1.6657 Angstrom
      mean = 1.6388 Angstrom
        t1 = 0.092752  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.061218  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T6  -- O14 = 1.6881 Angstrom
T6  -- O15 = 1.5706 Angstrom
T6  -- O16 = 1.6834 Angstrom
T6  -- O17 = 1.6416 Angstrom
      mean = 1.6459 Angstrom
        t1 = 0.061790  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.073180  (0.0 is a perfect tetrahedron)

        T-O SUMMARY
          Range  = 1.5542 A <--> 1.7434 A
          Mean   = 1.6378 A
          StdDev = 0.0526 A

       t1 Range  = 0.0497 <-- 0.0655 --> 0.0928
       t2 Range  = 0.0293 <-- 0.0609 --> 0.0828

-------------------------------------------------------------------
------------------------- O-T-O Analysis --------------------------
-------------------------------------------------------------------
O1  -- T1  -- O2  = 108.450 deg; O1  -- O2  = 3 A
O1  -- T1  -- O3  =  97.799 deg; O1  -- O3  = 2 A
O1  -- T1  -- O4  = 109.812 deg; O1  -- O4  = 3 A
O2  -- T1  -- O3  = 110.449 deg; O2  -- O3  = 3 A
O2  -- T1  -- O4  = 109.319 deg; O2  -- O4  = 3 A
O3  -- T1  -- O4  = 120.063 deg; O3  -- O4  = 3 A
       97.799 deg <-- 109.315 deg --> 120.063 deg

O3  -- T2  -- O5  = 102.089 deg; O3  -- O5  = 2 A
O3  -- T2  -- O6  = 125.184 deg; O3  -- O6  = 3 A
O3  -- T2  -- O7  = 100.011 deg; O3  -- O7  = 2 A
O5  -- T2  -- O6  = 105.470 deg; O5  -- O6  = 3 A
O5  -- T2  -- O7  = 113.579 deg; O5  -- O7  = 3 A
O6  -- T2  -- O7  = 110.519 deg; O6  -- O7  = 3 A
       100.011 deg <-- 109.475 deg --> 125.184 deg

O4  -- T3  -- O8  = 108.198 deg; O4  -- O8  = 3 A
O4  -- T3  -- O9  = 106.808 deg; O4  -- O9  = 3 A
O4  -- T3  -- O10 = 115.109 deg; O4  -- O10 = 3 A
O8  -- T3  -- O9  = 107.834 deg; O8  -- O9  = 3 A
O8  -- T3  -- O10 = 112.550 deg; O8  -- O10 = 3 A
O9  -- T3  -- O10 = 105.942 deg; O9  -- O10 = 3 A
       105.942 deg <-- 109.407 deg --> 115.109 deg

O6  -- T4  -- O7  = 101.251 deg; O6  -- O7  = 2 A
O6  -- T4  -- O11 = 119.086 deg; O6  -- O11 = 3 A
O6  -- T4  -- O12 =  98.126 deg; O6  -- O12 = 2 A
O7  -- T4  -- O11 = 100.544 deg; O7  -- O11 = 3 A
O7  -- T4  -- O12 = 114.045 deg; O7  -- O12 = 3 A
O11 -- T4  -- O12 = 122.499 deg; O11 -- O12 = 3 A
       98.126 deg <-- 109.259 deg --> 122.499 deg

O10 -- T5  -- O12 =  90.897 deg; O10 -- O12 = 2 A
O10 -- T5  -- O13 = 111.026 deg; O10 -- O13 = 3 A
O10 -- T5  -- O14 = 126.069 deg; O10 -- O14 = 3 A
O12 -- T5  -- O13 = 124.793 deg; O12 -- O13 = 3 A
O12 -- T5  -- O14 =  95.675 deg; O12 -- O14 = 2 A
O13 -- T5  -- O14 = 108.340 deg; O13 -- O14 = 3 A
       90.897 deg <-- 109.466 deg --> 126.069 deg

O14 -- T6  -- O15 =  99.755 deg; O14 -- O15 = 2 A
O14 -- T6  -- O16 = 121.840 deg; O14 -- O16 = 3 A
O14 -- T6  -- O17 = 110.385 deg; O14 -- O17 = 3 A
O15 -- T6  -- O16 = 103.957 deg; O15 -- O16 = 3 A
O15 -- T6  -- O17 = 105.791 deg; O15 -- O17 = 3 A
O16 -- T6  -- O17 = 112.739 deg; O16 -- O17 = 3 A
       99.755 deg <-- 109.078 deg --> 121.840 deg

        O-T-O SUMMARY
          Range  = 90.8967 deg <--> 126.0687 deg
          Mean   = 109.4512 deg
          StdDev = 8.8534 deg

        O--O SUMMARY
          Range  = 2.2963 A <--> 2.9844 A
          Mean   = 2.6694 A
          StdDev = 0.1779 A

-------------------------------------------------------------------
------------------------- T-T-T Analysis --------------------------
-------------------------------------------------------------------
-------------------------------------------------------------------
------------------------- T-O-T Analysis --------------------------
-------------------------------------------------------------------
T1  -- O1  -- T1  = 169.143 deg ; T1  -- T1   3.1515 A

T1  -- O2  -- T1  = 118.400 deg ; T1  -- T1   2.7862 A

T1  -- O3  -- T2  = 123.866 deg ; T1  -- T2   2.8841 A

T1  -- O4  -- T3  = 163.374 deg ; T1  -- T3   3.2806 A

T2  -- O5  -- T2  = 126.360 deg ; T2  -- T2   2.7938 A

T2  -- O6  -- T4  = 116.888 deg ; T2  -- T4   2.7672 A

T2  -- O7  -- T4  = 151.718 deg ; T2  -- T4   3.0453 A

T3  -- O8  -- T3  = 137.948 deg ; T3  -- T3   3.0870 A

T3  -- O9  -- T3  = 131.450 deg ; T3  -- T3   2.9679 A

T3  -- O10 -- T5  = 135.109 deg ; T3  -- T5   3.1514 A

T4  -- O11 -- T4  = 141.813 deg ; T4  -- T4   3.1825 A

T4  -- O12 -- T5  = 107.639 deg ; T4  -- T5   2.6445 A

T5  -- O13 -- T5  = 111.186 deg ; T5  -- T5   2.7541 A

T5  -- O14 -- T6  = 163.279 deg ; T5  -- T6   3.3181 A

T6  -- O15 -- T6  = 148.656 deg ; T6  -- T6   3.0244 A

T6  -- O16 -- T6  = 122.423 deg ; T6  -- T6   2.9504 A

T6  -- O17 -- T6  = 119.773 deg ; T6  -- T6   2.8402 A


        T-O-T SUMMARY
          Range  = 107.6386° <--> 169.1431 deg
          Mean   = 134.6486 deg
          StdDev = 18.5099 deg

        T--T SUMMARY
          Range  = 2.6445 A <--> 3.3181 A
          Mean   = 2.9782 A
          StdDev = 0.1932 A

-------------------------------------------------------------------
------------------------ *** WARNINGS *** -------------------------
-------------------------------------------------------------------

SOME OXYGEN ATOMS ARE TOO CLOSE TO EACH OTHER
O10 -- O12 = 2.2963 A

T-T-T analysis was not conducted.
T1  -- T1  = 2.7862 Angstrom
T2  -- T2  = 2.7938 Angstrom
T2  -- T4  = 2.7672 Angstrom

SOME T-ATOM DISTANCES ARE OUTSIDE THE NORMAL RANGE
T4  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T4  -- T2  = 2.7672 Angstrom
  T4  -- T4  = 3.1825 Angstrom
  T4  -- T5  = 2.6445 Angstrom
  T4  -- T6  = 3.2728 Angstrom
  T4  -- T2  = 3.0453 Angstrom
T5  -- T4  = 2.6445 Angstrom
T5  -- T5  = 2.7541 Angstrom
T6  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T6  -- T4  = 3.2728 Angstrom
  T6  -- T5  = 3.3181 Angstrom
  T6  -- T6  = 3.0244 Angstrom
  T6  -- T6  = 2.8402 Angstrom
  T6  -- T6  = 2.9504 Angstrom

-------------------------------------------------------------------
---------------------- Topological Analysis -----------------------
-------------------------------------------------------------------
T1 (Si): multiplicity = 24
Coordination Sequence =
    1 4 10 18 30 50 76 101 124 160 213 265 312 366 424 482 555
TD10 = 787
Circuit symbol = 4.5.4.5_{2}.6_{2}.7_{3}
Weight = 11
Vertex symbol  = 4.5.4.5_{2}.12.*
Weight = 20

T2 (Si): multiplicity = 24
Coordination Sequence =
    1 4 10 18 32 53 74 97 131 172 210 258 315 367 418 483 563
TD10 = 802
Circuit symbol = 4.5.4.6.5_{2}.6
Weight = 12
Vertex symbol  = 4.5.4.6.5_{2}.8
Weight = 17

T3 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 22 36 53 74 104 142 185 227 266 313 375 448 522 592
TD10 = 859
Circuit symbol = 4.6_{2}.5.6.6.7
Weight = 17
Vertex symbol  = 4.6_{2}.5.6.6.8
Weight = 22

T4 (Si): multiplicity = 24
Coordination Sequence =
    1 4 10 19 32 49 72 100 128 169 217 255 299 362 425 485 559
TD10 = 801
Circuit symbol = 4.6.4.6_{2}.5.6
Weight = 14
Vertex symbol  = 4.6_{2}.4.8.5.12
Weight = 24

T5 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 22 35 52 73 102 142 182 220 265 315 369 435 515 597
TD10 = 844
Circuit symbol = 4.5.6.8_{5}.6.8_{6}
Weight = 22
Vertex symbol  = 4.5.6.8_{3}.6.8_{4}
Weight = 22

T6 (Si): multiplicity = 24
Coordination Sequence =
    1 4 9 17 29 46 68 94 126 165 209 256 305 356 411 476 558
TD10 = 768
Circuit symbol = 4.6.4.6_{2}.4.6_{3}
Weight = 16
Vertex symbol  = 4.6.4.6_{2}.4.8
Weight = 20

<TD10> = 810.167
Average ring size = 5.5613
